Assessment of crystal quality and unit
cell orientation in epitaxial Cu
layers using polarized Raman scatteringChristoph Kr¨ammer,1,3,∗ Mario Lang,1,3Alex Redinger,2Johannes Sachs,1Chao Gao,1Heinz Kalt,1Susanne Siebentritt,2and Michael
1Institute of Applied Physics, Karlsruhe Institute of Technology (KIT), 76131 Karlsruhe,
2University of Luxembourg, Laboratory for Photovoltaics, Physics and Materials Science
Research Unit, L-4422 Belvaux, Luxembourg
3These authors contributed equally
Abstract: We use polarization-resolved Raman spectroscopy to assess the crystal quality of epitaxial kesterite layers. It is demonstrated for the example of epitaxial Cu2ZnSnSe4 layers on GaAs(001) that ”standing” and ”lying” kesterite unit cell orientations (c’-axis parallel / perpendicular to the growth direction) can be distinguished by the application of Raman tensor analysis. From the appearance of characteristic intensity oscillations when the sample is rotated one can distinguish polycrystalline and epitaxial layers. The method can be transferred to kesterite layers oriented in any crystal direction and can shed light on the growth of such layers in general.
© 2014 Optical Society of America
OCIS codes: (300.6450) Raman spectroscopy, (310.6870) Thin films, other properties.
References and links
1. W. Wang, M. T. Winkler, O. Gunawan, T. Gokmen, T. K. Todorov, Y. Zhu, and D. B. Mitzi, “Device characteris-tics of CZTSSe thin-film solar cells with 12.6% efficiency,” Adv. Energy Mater. 4, 1301465 (2013).
2. S. Oueslati, G. Brammertz, M. Buffi`ere, Thin Solid Films (submitted) (2014).
3. A. Redinger, R. Djemour, T. Weiss, J. Sendler, L. G¨utay, and S. Siebentritt, “Molecular beam epitaxy of Cu2ZnSnSe4thin films grown on GaAs(001),” in Proceedings of the 39th IEEE Photovoltaics Specialists
Con-ference(IEEE, 2013), pp.420–426.
4. C. Kr¨ammer, J. Sachs, M. Lang, L. Pfaffmann, C. Gao, D. Gerthsen, H. Kalt, M. Powalla, and M. Hetterich, “Fabrication of polycrystalline Cu2ZnSnSe4layers with strongly preferential grain orientation via selenization
of Sn/Cu/ZnSe(001)/GaAs(001) structures,” Appl. Phys. Lett. 104, 071913 (2014).
5. S. Siebentritt and S. Schorr, “Kesterites–a challenging material for solar cells,” Prog. Photovoltaics 20, 512–519 (2012).
6. S. Ahn, S. Jung, J. Gwak, A. Cho, K. Shin, K. Yoon, D. Park, H. Cheong, and J. H. Yun, “Determination of band gap energy (Eg) of Cu2ZnSnSe4thin films: On the discrepancies of reported band gap values,” Appl. Phys. Lett.
97, 021905 (2010).
7. M. Grossberg, J. Krustok, J. Raudoja, K. Timmo, M. Altosaar, and T. Raadik, “Photoluminescence and Ra-man study of Cu2ZnSn(SexS1−x)4monograins for photovoltaic applications,” Thin Solid Films 519, 7403–7406
8. M. Altosaar, J. Raudoja, K. Timmo, M. Danilson, M. Grossberg, J. Krustok, and E. Mellikov, “Cu2Zn1−xCdxSn(Se1−ySy)4 solid solutions as absorber materials for solar cells,” Phys. Status Solidi A 205,
9. R. Djemour, A. Redinger, M. Mousel, L. G¨utay, X. Fontan´e, V. Izquierdo-Roca, A. P´erez-Rodr´ıguez, and S. Siebentritt, “The three A symmetry Raman modes of kesterite in Cu2ZnSnSe4,” Opt. Express 21, A695–
10. R. Djemour, M. Mousel, A. Redinger, L. G¨utay, A. Crossay, D. Colombara, P. J. Dale, and S. Siebentritt, “De-tecting ZnSe secondary phase in Cu2ZnSnSe4by room temperature photoluminescence,” Appl. Phys. Lett. 102,
11. N. Vora, J. Blackburn, I. Repins, C. Beall, B. To, J. Pankow, G. Teeter, M. Young, and R. Noufi, “Phase iden-tification and control of thin films deposited by co-evaporation of elemental Cu, Zn, Sn, and Se,” J. Vac. Sci. Technol. A 30, 051201 (2012).
12. J. J. S. Scragg, L. Choubrac, A. Lafond, T. Ericson, and C. Platzer-Bj¨orkman, “A low-temperature order-disorder transition in Cu2ZnSnS4thin films,” Appl. Phys. Lett. 104, 041911 (2014).
13. M. Guc, S. Levcenko, V. Izquierdo-Roca, X. Fontan´e, E. Arushanov, and A. P´erez-Rodr´ıguez, “Polarized Raman scattering analysis of Cu2ZnSnSe4and Cu2ZnGeSe4single crystals,” J. Appl. Phys. 114, 193514 (2013).
14. D. Dumcenco and Y.-S. Huang, “The vibrational properties study of kesterite Cu2ZnSnS4single crystals by using
polarization dependent Raman spectroscopy,” Opt. Mater. 35, 419–425 (2012).
15. A. Redinger, D. M. Berg, P. J. Dale, and S. Siebentritt, “The Consequences of Kesterite Equilibria for Efficient Solar Cells,” J. Am. Chem. Soc. 133, 3320–3323 (2011).
16. B. Shin, Y. Zhu, N. A. Bojarczuk, S. Jay Chey, and S. Guha, “Control of an interfacial MoSe2 layer in
Cu2ZnSnSe4thin film solar cells: 8.9% power conversion efficiency with a tin diffusion barrier,” Appl. Phys.
Lett. 101, 053903 (2012).
17. R. Loudon, “The Raman effect in crystals,” Adv. Phys. 13, 423–482 (1964).
18. K. Momma and F. Izumi, “VESTA 3 for three-dimensional visualization of crystal, volumetric and morphology data,” J. Appl. Crystallogr. 44, 1272–1276 (2011).
19. T. G¨urel, C. Sevik, and T. C¸ a˘gın, “Characterization of vibrational and mechanical properties of quaternary com-pounds Cu2ZnSnS4and Cu2ZnSnSe4in kesterite and stannite structures,” Phys. Rev. B 84, 205201 (2011).
20. A. Khare, B. Himmetoglu, M. Johnson, D. J. Norris, M. Cococcioni, and E. S. Aydil, “Calculation of the lattice dynamics and Raman spectra of copper zinc tin chalcogenides and comparison to experiments,” J. Appl. Phys. 111, 083707 (2012).
In recent years, Cu2ZnSn(S,Se)4 has attracted increasing attention as a promising candi-date for sustainable thin-film photovoltaics. The structural similarity to the well-established Cu(In,Ga)(S,Se)2 (CIGS) and the absence of rare materials such as indium might be an im-portant step to sustainable thin-film photovoltaics in the future. However, achieved power-conversion efficiencies of 12.6 %  for the sulphoselenide and 10.4 %  for the pure Cu2ZnSnSe4(CZTSe) are still far below those of CIGS.
One key aspect to further improve the efficiency of CZTSe solar cells is a detailed under-standing of the physical properties of this complex material. Optical techniques such as modu-lation spectroscopy, time-resolved and temperature-dependent photoluminescence are powerful tools to gain insight into the band structure and carrier recombination mechanisms of CZTSe. However, in order to reach their full potential all of these techniques rely on high-quality sam-ples, preferentially single-crystalline and with a low amount of secondary phases.
Epitaxial samples can be fabricated using molecular-beam epitaxy  or a two-step ap-proach  on GaAs(001). The single crystalline substrate leads to a strong preferential orien-tation of the growing film. In the case of GaAs(001) the CZTSe layer is also oriented along the (001) orientation in contrast to polycrystalline absorbers grown on molybdenum coated soda lime glass which usually exhibit a dominant 112 peak (JCPDS-52-0868). However, due to the tetragonal kesterite unit cell with a c’/2a’-ratio of 0.996 (a’=5.695 ˚A, c’=11.345 ˚A)  there are three possible orientations when CZTSe is grown epitaxially on a cubic GaAs(001) substrate. One ”standing” (c’-axis k GaAs) and two ”lying” orientations (c’-axis k GaAs and GaAs, respectively) can be found, the two latter ones being equally probable due to the cu-bic symmetry of GaAs. The same situation can be found for the sulphide kesterite Cu2ZnSnS4 when grown on a cubic Si substrate. These different orientations can not be distinguished by X-ray diffraction (XRD).
Still, this technique holds a greater potential than mere phase identification. Using Raman spectroscopy, Scragg et al.  were able to show the preferential formation of ordered or disordered sulphidic kesterite under different annealing conditions. Guc et al.  determined the ratios of the elements of a Raman tensor which can be used to describe polarized Raman spectroscopy on CZTSe single crystals and Dumcenco et al.  studied CZTS samples with polarization-dependent Raman measurements.
Here, we analyze the crystallographic orientation for CZTSe epitaxial layers fabricated by two different techniques outlined below. As discussed in more detail later on, for epitaxially or-dered samples the intensity of the CZTSe Raman modes shows a characteristic behaviour when the sample is rotated around the optical axis. This behaviour depends on the kind of phonon mode one is observing but also on the grain orientations within the sample. In the example of CZTSe layers on GaAs(001), we show that the ”standing” kesterite unit cell orientation is prevalent and is independent of the fabrication route. Furthermore, the formalism can be trans-ferred to samples with an arbitrary crystallographic orientation.
2. Experiments and results
Epitaxial Cu2ZnSnSe4layers on GaAs(001) have been fabricated in a molecular-beam epitaxy (MBE) system via coevaporation of Cu, Zn, Sn, SnSe from effusion cells and Se from a valved cracker source at a nominal substrate temperature of 450◦C. The additional SnSe source is used to compensate for SnSe losses during growth . Further details of the growth process can be found in . In an alternative approach, strongly textured CZTSe samples are obtained using a two-step process. A Sn/Cu/ZnSe(001) stack is grown on GaAs(001) using MBE, and is then annealed in a selenium atmosphere. These layers show a strong preferential grain orientation in all three dimensions and can be seen as an intermediate step between real polycrystalline and fully epitaxial samples. Further details on the fabrication as well as the characterization of the samples can be found in . In the following, these samples will be referred to as textured sam-ples. For comparison, polycrystalline CZTSe samples have been fabricated by low-temperature coevaporation of elemental Cu,Zn,Sn and Se onto Mo-coated soda-lime glass (Mo/SLG) in the same MBE system where the precursors for the textured samples have been deposited, followed by selenization in a tube furnace. The process which is used is similar to that reported by Shin et al. .
Raman spectra are recorded using a frequency-doubled Nd:YVO4 laser (λ =532 nm) in a confocal excitation/detection setup. A double Fresnel rhomb is used to rotate the incoming linear polarization of the laser. Light is focused and scattered light from the sample is then collected using a microscope objective (20×, NA=0.4). The sample itself is mounted on a motorized rotation mount (MRM) and can be rotated around the optical axis (k GaAs direction). In the following, the corresponding angle of rotation will be referred to as α. After passing a razor-edge filter followed by a polarizer (analyzer) light is dispersed in a 0.46 m focal length monochromator using a 2400 l/mm grating. The spectra are then recorded using a charge-coupled device (CCD) camera.
Kesterite belongs to the space group I¯4, and Raman modes of 3 different symmetries–namely A,B and E–are possible. The different Raman tensors for this space group are given in Table 1 .
The intensity I of a Raman mode with a corresponding tensorR for incoming light of a given polarization eiand scattered light with a polarization esis proportional to
I ∝esTRei 2
Table 1. Raman tensors with tensor elements a-f for the space group I¯4 assuming a standing unit cell (z0|z k GaAs) 
RA= a 0 0 0 a 0 0 0 b RB(Z)= c d 0 d −c 0 0 0 0 RE(X)= 0 0 e 0 0 f e f 0 RE(Y)= 0 0 f 0 0 −e f −e 0
ei⊥esthe signal is represented by off-diagonal tensor elements. The different possible kesterite unit cell orientations can now be considered by applying the appropriate rotation matrices. For example, the Raman tensorsRAof the two lying unit cells are obtained by applying a rotation around the x- and y-axis of the laboratory system and are given by diag(a, b, a) and diag(b, a, a). The Raman tensors for B- and E-modes can be treated analogously. Again, it is important to note that the two possible lying kesterite unit cell orientations on GaAs(001) must occur simul-taneously due to the cubic structure of the substrate. In contrast, the lattice mismatch and the formation energy are slightly different for standing and lying kesterite due to the c’/2a’ ratio of 0.996 of the CZTSe unit cell. The intensity dependence of the Raman signal for a sample rotation around the optical axis can be described by a transformation of the Raman tensors using matrices for the rotation around the laboratory z-axis. Table 2 summarizes the resulting intensity dependencies on the rotation angle α for Raman modes of different symmetry and the two different polarizer configurations for a given set of tensor elements a-f (Unit cell pictures created using VESTA3 ).
For the lying kesterite the intensity contributions from both orientations add up to the re-sulting signal. Despite their mathematical complexity, all trigonometric expressions in Table 2 describe oscillations with a characteristic period of 90◦which essentially results from the sym-metry of the CZTSe unit cell. At this point, it is important to mention that a single lying unit cell orientation would result in an oscillation with a period of 180◦in the A and B-mode for eikes due to the reduced symmetry along the optical axis. However, the second lying unit cell yields the same oscillations but shifted by 90◦relative to the first orientation. In the end the coexis-tence of both lying configurations results in an oscillation with an effective period of 90◦. This means that all the oscillations described in Table 2 exhibit the same period of 90◦and are fur-ther in phase for one particular polarizer configuration. Furfur-thermore, the oscillations for eikes and ei⊥esare shifted by 45◦relative to each other which means that they are opposite in phase. Again, we note that–by using appropriate transformation matrices–this formalism can be trans-ferred to analyze kesterite layers with an arbitrary crystal orientation, e.g., Cu2ZnSnS4(112) on Si(111).
On the other hand, for a randomly oriented ensemble of unit cells (as found in fully polycrys-talline samples), no intensity oscillations are expected, since contributions from all different possible orientations average out. This fact can be used to verify that the oscillations occuring in our experiments are no measurement artifacts.
Table 2. Angular intensity dependencies for sample rotation around the optical axis for the different CZTSe unit cell orientations on GaAs(001).
Unit cell orientation Symmetry eikes ei⊥es
A ∝ |a|2 0
B ∝ |c(cos2α − sin2α ) + 2d sin α cos α |2 ∝ |d(cos2α − sin2α ) − 2c sin α cos α |2
E 0 0
c‘ c‘ A ∝ |a cos2α + b sin2α |2+ |b cos2α + a sin2α |2 ∝ 2(a − b)2cos2α sin2α
B ∝ c2(cos4 α + sin4α ) ∝ 2c2cos2 α sin2α E ∝ 4(e2+ f2) cos2 α sin2α ∝ (e2+ f2)(cos2 α − sin2α )2 at around 80 cm−1.
However, the theoretical intensity oscillations for a sample rotation do not change qualita-tively in terms of period or phase depending on the mode symmetry (B or E), since in our experiment the optical axis coincides with the highly symmetrical CZTSe directions ( or  or ). Besides, the scope of this article is not to accurately determine the symmetry of the occurring Raman modes but instead to detect a preferential unit cell orientation within the thin film and to judge the crystal quality.
Figure 2 shows the observed angular intensity dependence of the different samples for both the kesterite A-mode at 197 cm−1 and the CZTSe mode at around 80 cm−1. All Raman in-tensities were measured in the peak maximum and normalized to the intensity of the CZTSe A-mode at 197 cm−1(eikes). The randomly orientated polycrystalline sample does not exhib-it any angular intensexhib-ity dependence. Fluctuations in the signal do not exhibexhib-it any periodicexhib-ity and are purely due to an inhomogeneous sample quality. This is consistent with the theoretical expectation that all contributions from randomly orientated grains average out. Furthermore, this result confirms that the observed oscillations for the other samples are not an artifact of the measurement.
In contrast to that, both the textured and the epitaxial sample exhibit a clear angular intensity dependence. For the CZTSe mode around 80 cm−1 an oscillation with a period of 90◦is ob-served for both polarizer configurations. As expected, the oscillations are opposite in phase for the two different polarizations. These findings prove the strong preferential orientation of unit
0 . 0 0 . 2 0 . 4 0 . 6 0 . 8 1 . 0 0 . 0 0 . 2 0 . 4 0 . 6 0 . 8 1 . 0 0 . 0 0 . 2 0 . 4 0 . 6 0 . 8 1 . 0 0 9 0 1 8 0 2 7 0 3 6 0 0 . 0 8 0 . 1 2 0 . 1 6 0 9 0 1 8 0 2 7 0 3 6 0 0 . 0 8 0 . 1 2 0 . 1 6 0 9 0 1 8 0 2 7 0 3 6 0 0 . 0 8 0 . 1 2 0 . 1 6 ei | | es ei⊥ es 1 9 7 c m -1 N o rm . In te n s it y A A 0 0 1 8 ei | | es ei⊥ es A A 0 0 2 4 ei| | es ei⊥ es ei| | es ei⊥ es A R 2 9 6 ei| | es ei⊥ es S a m p l e R o t a t i o n ( ° ) 8 0 c m -1 N o rm . In te n s it y A A 0 0 1 8 P o l y c r y s t a l l i n e S a m p l e T e x t u r e d S a m p l e E p i t a x i a l S a m p l e ei| | es ei⊥ es S a m p l e R o t a t i o n ( ° ) A A 0 0 2 4 S a m p l e R o t a t i o n ( ° ) A R 2 9 6
Fig. 2. Intensity dependence under sample rotation for three different samples. The poly-crystalline sample does not exhibit any oscillations whereas the epitaxial samples exhibit intensity oscillations with a period of 90◦. The intensity behaviour of the A-mode indicates the presence of lying kesterite unit cells on the GaAs substrate. Intensities were normalized to the A-mode at 197 cm−1(eikes).
cells within the sample. The kesterite modes at around 249 cm−1exhibit the same behaviour qualitatively under sample rotation which is why they are not shown separately in this letter.
Interestingly, for eikesthe kesterite A-modes of the textured and the epitaxial CZTSe sample show an almost constant intensity under sample rotation which is consistent with theory for standing kesterite unit cells. However, slight intensity oscillations are visible. Furthermore, for ei⊥es we observe an intensity oscillation instead of a vanishing signal. This confirms the existence of lying kesterite unit cells within the film. We conclude that the majority of unit cells is of standing orientation on GaAs due to the constant A-mode intensity under sample rotation for eikes. This majority of standing unit cells is then blocked out when ei⊥es, and the remaining oscillating signal is originating from the minority of lying unit cells. For eikes the resulting oscillation for a mixture of standing (constant intensity) an lying (oscillating intensity) unit cells is probably masked by sample inhomogeneities on the surface. In addition, an increasing contrast between the A-mode intensity for eikes and ei⊥es can be observed when looking at the transition in crystallinity for those three samples going from left to right in Fig. 2. One way to interprete this finding is that the amount of polycrystalline inclusions with a different grain orientation is further reduced in the epitaxial sample compared to the textured sample.
Again, the behaviour of the second A-mode at 172 cm−1is qualitatively identical to the Ra-man mode at 197 cm−1and is therefore not shown either. Since the presence of a stannite phase cannot be excluded within the sample it is important to note that the Raman tensor of the corre-sponding stannite A1-mode is identical in shape with that of a kesterite A-mode. Accordingly, the same intensity behaviour results for the different unit cell orientations. This means that the conclusions which were drawn about the unit cell orientation also hold for stannite CZTSe on GaAs(001).
crystalline orientation for both epitaxial and textured layers. This means, that–due to the finite penetration depth of the laser and the small spot size–polarized Raman spectroscopy is able to detect sample inhomogeneities with a higher spatial resolution than XRD analysis.
In conclusion, Raman spectroscopy has been used to assess the crystallographic orientation in CZTSe samples. Clear intensity oscillations evolve from a constant signal under sample rota-tion when the unit cell order within the films is increased. This has been shown experimentally by analyzing three different types of sample crystallinities going from a randomly oriented en-semble of unit cells in a polycrystalline CZTSe layer on Mo/SLG to a textured layer and an epitaxial layer on GaAs(001). Furthermore, it has been shown that the observed intensity oscil-lations cannot be due to purely standing kesterite unit cells on GaAs. These findings confirm that polarized Raman spectroscopy can be used to easily access unit cell orientations within high-quality CZTSe layers and additionally grants high spatial resolution. By analyzing the intensity contrast between the different polarizer configurations it is possible to obtain infor-mation about the degree of texture by comparison of different samples. The analysis can be extended to investigate kesterite layers with an arbitrary crystal orientation to determine crys-tallinity and unit cell orientation.